infiltration and percolation
Post on 23-Dec-2015
Embed Size (px)
Infiltration And PercolationReporters:Petalio, Paul B.Regala, Mark Gerald P.Salonga, Jason R
10th International Conference on Concrete Block Paving Shanghai, Peoples Republic of China, November 24-26, 2012
Potential Application of ASTM C 1701 for Evaluating Surface Infiltration of Permeable Interlocking Concrete Pavements
David R. Smith Kevin Earley Justin M. Lia
Introduction Permeable interlocking concrete pavement (PICP) has seen increased use for stormwater management and low impact development (LID). Surface infiltration is a key performance indicator for surface cleaning using vacuum equipment.This paper provides background on the development of test methods for measuring surface infiltration of permeable pavements. Among those test methods is the single ring infiltrometer described in ASTM C 1701 Standard Test Method for Infiltration Rate of In Place Pervious Concrete. This test method was initially developed to measure surface infiltration of PICP and concrete grid pavements in 2004, and approved and published by American Society for Testing and Materials (ASTM) in 2009 as a test method only for pervious concrete.
Review and Assessment of Existing StudyIn 2004, ASTM D 3385 was tried by Bean (Bean 2007) while evaluating surface infiltration of PICP, concrete grid and pervious concrete pavement sites in North Carolina, Virginia, Maryland, and Delaware. He moved to a single ring infiltrometer due to high surface infiltration rates of the permeable pavements tested and the volume of water required for maintaining hydraulic heads within the rings. Bean reports test results from 14 PICP sites using a single ring device sealed with plumbers putty to the pavement surface. He measured values between 1.1 x 10-2 m/sec and 4.4 x 10-6 m/sec on PICP. The lowest values were due to clogging from fines, i.e., sediment on the surface. Values between 1.9 x 10-2 and 3 x 10-5 m/sec were measured on pervious concrete, again with the lowest values due to clogging from fines.
Jennifer Drake, a doctoral student with the University of Guelph is conducting a series of surface infiltration tests on PICP and pervious concrete sites in Ontario, Canada using ASTM C 1701 as well double ring test methods. She is also investigating water volume and pollutant removal from these pavements. Her observations regarding both pavement types are that they require regular vacuum sweeping in order to maintain surface infiltration rates. She noted at an October 2011 presentation in Ontario (Drake 2011) that for hot weather (over 30 C.), non-oil base modeling clay works better than plumbers putty as the latter material becomes viscous, stringy, and difficult to handle. The modeling clay molds quickly and creates a seal between the ring and pavers
Issues and ConcernPermeability of Conventional ConcreteFlooding of Impervious Characteristics of Conventional ConcreteRainwater is Suspended on Surface of Concrete Instead of Penetrating to Ground Surface
Good Practices Related to the TopicInnovation of Pervious Concrete Design Mix
Possible SolutionsApplication of Pervious Concrete as a Pavement StructureDevelopment of the Design of Permeable Concrete
Recommended SolutionsConduct More Studies on Pervious Concrete
ObjectivesTo Know What is Pervious Concrete its PropertiesTo Know its Effectiveness as Permeable Material
Detailed DescriptionThere are several ways to assess infiltration of rainfall and runoff into permeable pavements. In ascending cost order they include: (1) visual inspection during or immediately after a rainstorm for ponding; (2) measuring surface infiltration on sampled small areas; (3) generating synthetic rainfall and runoff for a distinct rain event which often involves a rain simulator; and (4) continuous monitoring of rainfall and surface runoff usually over a period years. The PICP and pervious concrete pavement industries elected to use method (2) i.e., sampling and testing the surface infiltration rate of small areas across a larger pavement for acceptance testing of newly constructed pavements as well as for assessing in-service surface infiltration. This test method is formalized in ASTM C 1701. The test method was proposed by the pervious concrete industry. The selection of this testing approach is likely due to the speed and economy of conducting tests in this manner .
TerminologiesPervious Concrete - (also called porous concrete, permeable concrete, no fines concrete and porous pavement) is a special type of concrete with a highporosity used for concrete flatwork applications that allows water from precipitationand other sources to pass directly through, thereby reducing the runoff from a site and allowing groundwater recharge.Infiltration - is the process by whichwateron the ground surface enters the soil.Percolation - the movement of water downward and radially through the subsurface soil layers, usually continuing downward to the groundwater.PICP - permeable interlocking concrete pavements
Scope of the StudyDesign Mix of the Pervious ConcreteDetermination of the Properties of Pervoius Concrete as a Material
Design AnalysisPICP Infiltration Tests in New York To further demonstrate the utility of this test method for PICP, results from two sites from 4Site Engineering in 2010 and 2011 are provided (Lia 2011 and Lia 2011b). Both sites are in Lindenhurst, New York, the first being an 880 m2 parking lot at a building materials supply store. The paving units were 120 x 225 x 80 mm thick with 13 mm joints filled with a stone gradation conforming to ASTM No. 9 stone per ASTM D448 Standard Classification for Sizes of Aggregate for Road and Bridge Construction. For ASTM No. 9 aggregate, stone sizes range from 4.75 to 0.30 mm. According to The Aggregate Handbook (NSA 1991), this material has a hydraulic conductivity of at least 3.5 x 10-3 m/sec.
The paving units and jointing material were installed over 40 mm thick ASTM No. 8 bedding stone. This aggregate is slightly larger in size than the ASTM No. 9 stone in the paver joints. This bedding stone was placed over a 100 mm thick ASTM No. 57 base over a 675 mm thick subbase of ASTM No. 3 stone. ASTM No. 57 base ranges in size from 25 to 2.36 mm and ASTM No. 3 is 50 down to 12.5 mm. Both test locations in Lindenhurst used plumbers putty to seal the metal ring against the pavers as shown in Figure 2. On both sites, the jointing stones are removed between the joints under the ring and filled with plumbers putty to further direct the water downward. Removal of the jointing stones can be done with a putty knife and screwdriver. A key consideration on locating the ring is to frame the paver joint pattern within the ring. This framed area should represent the percentage of open area in the overall surface to best characterize surface infiltration. Besides characterizing the overall permeable jointing pattern, this location can reduce the time and effort required to remove jointing stones and filling the joints with plumbers putty.
ASTM C1701 test apparatus at a building supply store parking lot
Technical SpecificationsAfter pre-wetting, ASTM C 1701 test method was conducted three times over the first 11 months of service that resulted in an average infiltration rate of 2.025 x 10-3 m/sec or 287 in./hr. Table 1 provides the test data for three test locations. Table 1. PICP test results for a building supply parking lot in Lindenhurst, New York, in m/sec Table 1. PICP test results for a building supply parking lot in Lindenhurst, New York, in m/sec
Another test using ASTM C1701 was conducted at a 600 m2 PICP parking lot at a public library in Lindenhurst, New York. The paving units were 200 x 200 x 80 mm thick with 13 mm wide joints filled with ASTM No. 8 stone. The paving units and jointing material were installed over 40 mm thick ASTM No. 8 bedding stone. This was placed over a 100 mm thick ASTM No. 57 base and a 150 mm thick subbase of ASTM No. 3 stone over a highly permeable soil subgrade.
ASTM C1701 test apparatus at a public library parking lot
After pre-wetting (i.e., applying water without measurements) the ASTM C 1701 test method was conducted in April, 2011 during the first months of service that resulted in an average infiltration rate of 3.8 x 10-3 m/sec.
PICP test results for a public library parking lot in Lindenhurst, New York, in m/sec
Conclusions And RecommendationsThe most common permeable pavement surfaces are pervious concrete, PICP and porous asphalt. There are millions of square meters of each in service. ASTM C 1701 is an inexpensive and rapid test method for measuring surface infiltration by simulating a small hydraulic head on the surface test area like those generated by intense rain storms and contributing runoff. Data and experience from Bean, Lia, and Drake confirm that C1701 is suitable for testing the surface infiltration of PICP and Bean extends its use to successfully testing concrete grid pavements. Borst reports using a modified version of C 1701 to test PICP, pervious concrete, and porous asphalt as part of a nationally visible evaluation of these pavements.
In order for contractors, stormwater agencies and project owners to better understand performance of maintenance needs of all permeable pavements, ASTM C 1701 should be revised to address PICP, concrete grid pavements, and porous asphalt testing. Chopra 2010 and Vancura 2010 demonstrate that permeable pavements can experience a reduction in their surface infiltration rates especially if not maintained with vacuum sweeping. Broadening the application of ASTM C 1701 to characterize the surface infiltration of more than just pervious concrete enables an objective comparison of the performance other pavement systems designed to reduce stormwater runoff.
ASTM C 170